(a) anodic inhibitors: phosphates
(b) Cathodic inhibitorspoly-phosphates Ca(HCO3)2methylamino-phosphate
(c) mixed anodic and cathodic inhibitorsaminesselenides
Types of Corrosion Inhibitors
OrganicThese materials are characterized by high molecular weight structures, incorporating nitrogen or phosphorous groups. They are usually highly polar molecules.
InorganicSalts of some metals and amphoteric elements act as corrosion inhibitors. Quite often these materials have tenacious filmforming or passivation effects. In some instances, they react with the metal surface.
Chromate SaltsZinc SaltsMolybdate Compounds Phosphates Nitrite SaltsSilicate Compounds
Adsorption of organic inhibitor onto a metal surface in aqueous environment
The percentage inhibitor efficiency is �given by:
where Wo and Wi represent weight loss in the absence and presence of inhibitor, respectively.
Mild steel corrosion rate in 2.0 M HCl in the presence and absence of inhibitor
Mechanism of inhibition
According to Bockris and Drazic, the inhibition mechanism can be explained by the Fe±(Inh)ads reaction intermediates
This Fe-(Inh)ads intermediate forms an adsorption layer through the nitrogen atom of the inhibitor. The adsorption layer acts as a hindrance to the solution and enhances the protection of the metal surface.
The adsorption of an organic compound on the surface of a mild steel electrode is regarded as a substitutional adsorption process between the organic compound in the aqueous phase (Orgad) and the water molecules adsorbed on the mild steel surface (H2Oad)
where X is the size ratio, that is, the number of water molecules replaced by one organic molecule.
The degree of surface coverage θ can be plotted as a function of the concentration of hexylamine or dodecylamine inhibitors in the hydrochloric acid solution. The value of θ wascalculated from the inhibitor eciency relationship� :
Adsorption isothermInteraction between the organic compounds and metal surfaces
Adsorption isotherm plots
The most commonly used substitutional isotherms:
H.P. Dhar, B.E. Conway and K.M. Joshi, Electrochim. Acta 18 (1973) 789.Flory-Huggins
Bockris-SwinkelsJ. O'M. Bockris and D.A.J. Swinkels, J. Electrochem. Soc. 111 (1964) 736.
H.P. Dhar, B.E. Conway and K.M. Joshi, Electrochim. Acta 18 (1973) 789.
where X is the number of water molecules replaced by one molecule of organic compound, c is the inhibitor concentration and k is the equilibrium constant of the adsorption reaction given by: kc = 1/55.5[exp(-Gads
Equations at the top may be written as:
where f (θ, X) is the configurational term, which depends essentially on the physical model and assumptions underlying the derivation of the isotherm .
J.M. BASTIDAS, J.L. POLO and E. CANO , Journal of Applied Electrochemistry 30: 1173±1177, 2000.
Flory-Huggins isotherm plot Bockris-Swinkels isotherm plot
A plot of log f (θ, X) against log c, for a specified value of X, is a straight line with a slope of unity, and the ordinate axis intercept gives the log k value.
the area occupied by a vertically-oriented adsorbed hexylamine/dodecylamine molecule is about 17 A o 2 (the projected area of a rectangle surrounding a molecule), as compared with 50 A o 2 for hexylamine and 85 A o 2 for dodecylamine for the horizontal orientations
Two kinds of adsorption can be acting on steel surface:
Type A means the interaction between the benzene ring, C N and the vacant, low energy d-orbitals of Fe surface atoms, this process is called chemisorption. Type B shows theelectrostatic interaction between the positively charged N atom and the negatively charged Cl− on mild steel surface, which is regard as physisorption.
Weihua Li a, , Qiao Heb, Changling Pei c, Baorong Houa∗ , Electrochimica Acta 52 (2007) 6386–6394
Applied Surface Science 236 (2004) 155–164M. Özcan, I˙. Dehri, M. Erbil,
A vapor phase corrosion inhibitor is used to protect the annular space in road crossings.
Below ground road casing. Annular space between the casing and the carrier pipe can be protected with a VpCI or filled to mitigate corrosion in the annular space.
Application of corrosion inhibitors
Engine coolants Sodium chromateFe, Pb, Cu,
.. Sodium nitrite Fe 0.1-1%
.. Borax .. 1%
Glycol/water Borax + MBT All 1% + 0.1%
Oil field brines Sodium silicate Fe 0.01%
.. Quaternaries .. 10-25 ppm
.. Imidazoline .. 10-25ppm
Seawater Sodium silicate Zn 10 ppm
.. Sodium nitrite Fe 0.5%
.. Calcium bicarbonate All pH dependent
.. Sodium phosphate monobasic + Sodium nitrite Fe 10 ppm + 0.5%
Application of corrosion inhibitors
System Inhibitor Metals Concentration AcidsHCl Ethylaniline Fe 0.5%
.. Mercaptobenzotriazole .. 1%
.. Pyridine + phenylhydrazine .. 0.5% + 0.5%
.. Rosin amine + ethylene oxide .. 0.2% Sulfuric Phenylacridine .. 0.5%
Phosphoric Sodium iodide .. 200 ppm Others Thiourea .. 1%
.. Sulfonated castor oil .. 0.5-1.0%
.. Arsenic Oxide .. 0.5%
.. Sodium arsenate .. 0.5% Water
Potable Calcium bicarbonate Steel, cast iron 10 ppm
.. Polyphosphate Fe, Zn, Cu, Al 5-10 ppm
.. Calcium hydroxide Fe, Zn, Cu 10 ppm
.. Sodium silicate .. 10-20 ppm
Cooling Calcium bicarbonate Steel, cast iron 10 ppm
.. Sodium chromate Fe, Zn, Cu 0.1%
.. Sodium nitrite Fe 0.05%
.. Sodium phosphate monobasic .. 1%
.. Morpholine .. 0.2% Boilers Sodium phosphate monobasic Fe, Zn, Cu 10 ppm
.. Polyphosphate .. 10 ppm
.. Morpholine Fe variable
.. Hydrazine .. O2 scavenger
.. Ammonia .. neutralizer
.. Octadecylamine .. variable